High intensity QTH light sources 20. Uhl A, Mills RW, Rzanny AE, Jandt KD. Time dependence of composite shrinkage using halogen and LED light curing. Dent Mater 2005;21:278-286. 21. Felix CA, Price RB, Andreou P. Effect of reduced exposure times on the microhardness of 10 resin composites cured by high-power LED and QTH curing lights. J Can Dent Assoc 2006;72:147. 22. Asmussen E. Restorative resins: hardness and strength vs. quantity of remaining double bonds. Scand J Dent Res 1982;90:484-489. 23. Ferracane JL. Correlation between hardness and degree of conversion during the setting reaction of unfilled dental restorative resins. Dent Mater 1985;1:11-14. 24. Johnston WM, Leung RL, Fan PL. A mathematical model for post-irradiation hardening of photoactivated composite resins. Dent Mater 1985;1:191-194. 25. DeWald JP, Ferracane JL. A comparison of four modes of evaluating depth of cure of light-activated composites. J Dent Res 1987;66:727-730. 26. Aravamudhan K, Floyd CJ, Rakowski D, Flaim G, Dickens SH, Eichmiller FC, Fan PL. Light-emitting diode curing light irradiance and polymerization of resin-based com- posite. J Am Dent Assoc 2006;137:213-223. 27. Ernst CP, Meyer GR, Muller J, Stender E, Ahlers MO, Wil- lershausern B. Depth of cure of LED vs QTH light-curing devices at a distance of 7 mm. J Adhes Dent 2004;6:141-150. 28. Cook WD. Spectral distributions of dental photopolymer- ization sources. J Dent Res 1982;61:1436-1438. 29. Besnault C, Pradelle-Plasse N, Picard B, Colon P. Effect of a LED versus halogen light cure polymerization on the curing characteristics of three composite resins. Am J Dent 2003;16:323-328. 30. Nomoto R, McCabe JF, Hirano S. Comparison of halogen, plasma and LED curing units. Oper Dent 2004;29:287-294. 31. Miyazaki M, Oshida Y, Moore BK, Onose H. Effect of light exposure on fracture toughness and flexural strength of light-cured composites. Dent Mater 1996;12:328-332. 32. Baharav H, Abraham D, Cardash HS, Helft M. Effect of exposure time on the depth of polymerization of a visible light-cured composite resin. J Oral Rehabil 1988;15:167- 172. 33. Mills RW, Jandt KD, Ashworth SH. Dental composite depth of cure with halogen and blue light emitting diode technol- ogy. Br Dent J 1999;186:388-391. 34. Kurachi C, Tuboy AM, Magalhaes DV, Bagnato VS. Hard- ness evaluation of a dental composite polymerized with experimental LED-based devices. Dent Mater 2001;17:309- 315. 304 European Journal of Dentistry 35. Tarle Z, Knezevic A, Demoli N, Meniga A, Sutaloa J, Unter- brink G, Ristic M, Pichler G. Comparison of composite cur- ing parameters: effects of light source and curing mode on conversion, temperature rise and polymerization shrink- age. Oper Dent 2006;31:219-226. 36. Kawaguchi M, Fukushima T, Miyazaki K. The relationship between cure depth and transmission coefficient of visible- light-activated resin composites. J Dent Res 1994;73:516- 521. 37. Guiraldo RD, Consani S, Lympius T, Schneider LF, Sinho- reti MA, Correr-Sobrinho L. Influence of the light curing unit and thickness of residual dentin on generation of heat during composite photoactivation. J Oral Sci 2008;50:137- 142. 38. Bouillaguet S, Caillot G, Forchelet J, Cattani-Lorente M, Wataha JC, Krejci I. Thermal risks from LED- and high- intensity QTH-curing units during polymerization of dental resins. J Biomed Mater Res B Appl Biomater 2005;72:260-267. 39. Stewardson DA, Shortall AC, Harrington E, Lumley PJ. Thermal changes and cure depths associated with a high intensity light activation unit. J Dent 2004;32:643-651.